#------------------------------------------------------------------------------
#$Date: 2019-10-13 11:52:27 +0300 (Sun, 13 Oct 2019) $
#$Revision: 219318 $
#$URL: file:///home/coder/svn-repositories/cod/cif/3/00/02/3000248.cif $
#------------------------------------------------------------------------------
#
# This file is available in the Crystallography Open Database (COD),
# http://www.crystallography.net/
#
# All data on this site have been placed in the public domain by the
# contributors.
#
data_3000248
loop_
_publ_author_name
'Auer, Henry'
'Yang, Fangshun'
'Playford, Helen Y.'
'Hansen, Thomas C.'
'Franz, Alexandra'
'Kohlmann, Holger'
_publ_section_title
;
 Covalent Si--H Bonds in the Zintl Phase Hydride CaSiH1+x (x ≤ 1/3)
;
_journal_issue                   9
_journal_name_full               Inorganics
_journal_page_first              106
_journal_paper_doi               10.3390/inorganics7090106
_journal_volume                  7
_journal_year                    2019
_chemical_formula_sum            'Ca D0.09 Si'
_chemical_formula_weight         68.36
_space_group_IT_number           63
_space_group_name_Hall           '-C 2c 2'
_space_group_name_H-M_alt        'C m c m'
_symmetry_cell_setting           orthorhombic
_symmetry_space_group_name_Hall  '-C 2c 2'
_symmetry_space_group_name_H-M   'C m c m'
_cell_angle_alpha                90
_cell_angle_beta                 90
_cell_angle_gamma                90
_cell_formula_units_Z            4
_cell_length_a                   4.5391(6)
_cell_length_b                   10.9521(15)
_cell_length_c                   3.9028(6)
_cell_measurement_temperature    529
_cell_volume                     194.02(5)
_computing_structure_refinement  TOPAS
_diffrn_ambient_temperature      529
_diffrn_measurement_device_type
;
   'D20'
;
_diffrn_radiation_monochromator  'Ge 115'
_diffrn_radiation_type           neutron
_diffrn_radiation_wavelength     1.86829
_diffrn_source                   'nuclear reactor'
_diffrn_source_type              D20
_exptl_crystal_density_diffrn    2.340
_pd_char_colour                  grey
_pd_instr_location               'D20 diffractometer, ILL, Grenoble, France'
_pd_meas_2theta_range_inc        0.02
_pd_meas_2theta_range_max        140
_pd_meas_2theta_range_min        5
_pd_proc_2theta_range_inc        0.02
_pd_proc_2theta_range_max        122
_pd_proc_2theta_range_min        8
_pd_proc_ls_prof_R_factor        6.00
_pd_proc_ls_prof_wR_expected     4.48
_pd_proc_ls_prof_wR_factor       7.69
_pd_proc_wavelength              1.86829
_pd_spec_mounting                'sapphire single crystal cell'
_pd_spec_shape                   cylinder
_pd_spec_size_axial              10
_pd_spec_size_equat              6
_refine_ls_goodness_of_fit_all   1.72
_refine_ls_number_parameters     26
_refine_ls_number_reflns         58
_refine_ls_number_restraints     0
_refine_ls_R_I_factor            6.21
_refine_ls_shift/su_max          0.05
_cod_data_source_file            CaSiD0.092_ILL.cif
_cod_data_source_block           CaSiD0.092
_cod_depositor_comments
'Releasing structure 3000248 into public domain as published material.'
_cod_original_sg_symbol_H-M      Cmcm
_cod_original_formula_sum        'Ca D0.09 Si1'
_cod_database_code               3000248
loop_
_symmetry_equiv_pos_as_xyz
'x, y, z '
'-x, -y, z+1/2 '
'-x, y, -z+1/2 '
'-x, y, z '
'x, -y, -z '
'x, -y, z+1/2 '
'x, y, -z+1/2 '
'-x, -y, -z '
'x+1/2, y+1/2, z '
'-x+1/2, -y+1/2, z+1/2 '
'-x+1/2, y+1/2, -z+1/2 '
'-x+1/2, y+1/2, z '
'x+1/2, -y+1/2, -z '
'x+1/2, -y+1/2, z+1/2 '
'x+1/2, y+1/2, -z+1/2 '
'-x+1/2, -y+1/2, -z '
loop_
_atom_site_label
_atom_site_type_symbol
_atom_site_symmetry_multiplicity
_atom_site_fract_x
_atom_site_fract_y
_atom_site_fract_z
_atom_site_occupancy
_atom_site_B_iso_or_equiv
Ca1 Ca 4 0 0.3592(5) 0.25 1 2.82(11)
Si1 Si 4 0 0.0726(5) 0.25 1 2.82(11)
D D 4 0.5 0.266(4) 0.25 0.092(5) 2.82(11)
loop_
_atom_type_symbol
_atom_type_scat_length_neutron
_atom_type_scat_source
Ca 0.470 V.F._Sears_Neutron_News_3_26_(1992)
Si 0.41491 V.F._Sears_Neutron_News_3_26_(1992)
D 0.667 V.F._Sears_Neutron_News_3_26_(1992)
loop_
_geom_angle_atom_site_label_1
_geom_angle_atom_site_label_2
_geom_angle_atom_site_label_3
_geom_angle
_geom_angle_site_symmetry_1
_geom_angle_site_symmetry_2
_geom_angle_site_symmetry_3
D Ca1 D 110.0(16) 10_554 1_555 10_555
D Ca1 D 76.3(2) 1_555 1_555 10_554
D Ca1 D 76.3(2) 1_555 1_555 10_555
D Ca1 D 131.4(18) 1_455 1_555 1_555
D Ca1 D 76.3(2) 1_455 1_555 10_554
D Ca1 D 76.3(2) 1_455 1_555 10_555
Si1 Ca1 D 55.2(6) 10_455 1_555 1_455
Si1 Ca1 D 140.37(12) 10_455 1_555 1_555
Si1 Ca1 D 131.1(2) 10_455 1_555 10_554
Si1 Ca1 D 67.7(5) 10_455 1_555 10_555
Si1 Ca1 Si1 152.0(3) 10_554 1_555 10_455
Si1 Ca1 D 140.37(12) 10_554 1_555 1_455
Si1 Ca1 D 55.2(6) 10_554 1_555 1_555
Si1 Ca1 D 67.7(5) 10_554 1_555 10_554
Si1 Ca1 D 131.1(2) 10_554 1_555 10_555
Si1 Ca1 Si1 94.73(7) 10_454 1_555 10_554
Si1 Ca1 Si1 78.47(5) 10_454 1_555 10_455
Si1 Ca1 D 55.2(6) 10_454 1_555 1_455
Si1 Ca1 D 140.37(12) 10_454 1_555 1_555
Si1 Ca1 D 67.7(5) 10_454 1_555 10_554
Si1 Ca1 D 131.1(2) 10_454 1_555 10_555
Si1 Ca1 Si1 152.0(3) 10_555 1_555 10_454
Si1 Ca1 Si1 78.47(5) 10_555 1_555 10_554
Si1 Ca1 Si1 94.73(7) 10_555 1_555 10_455
Si1 Ca1 D 140.37(12) 10_555 1_555 1_455
Si1 Ca1 D 55.2(6) 10_555 1_555 1_555
Si1 Ca1 D 131.1(2) 10_555 1_555 10_554
Si1 Ca1 D 67.7(5) 10_555 1_555 10_555
Si1 Ca1 Si1 104.02(14) 1_555 1_555 10_555
Si1 Ca1 Si1 104.02(14) 1_555 1_555 10_454
Si1 Ca1 Si1 104.02(14) 1_555 1_555 10_554
Si1 Ca1 Si1 104.02(14) 1_555 1_555 10_455
Si1 Ca1 D 65.7(9) 1_555 1_555 1_455
Si1 Ca1 D 65.7(9) 1_555 1_555 1_555
Si1 Ca1 D 55.0(8) 1_555 1_555 10_554
Si1 Ca1 D 55.0(8) 1_555 1_555 10_555
Si1 Si1 Si1 101.7(4) 2_554 1_555 2_555
D Si1 Si1 81.4(7) 10_554 1_555 2_554
D Si1 Si1 176.9(7) 10_554 1_555 2_555
D Si1 D 95.5(14) 10_555 1_555 10_554
D Si1 Si1 176.9(7) 10_555 1_555 2_554
D Si1 Si1 81.4(7) 10_555 1_555 2_555
Ca1 Si1 D 50.9(2) 10_455 1_555 10_555
Ca1 Si1 D 107.8(5) 10_455 1_555 10_554
Ca1 Si1 Si1 130.05(15) 10_455 1_555 2_554
Ca1 Si1 Si1 70.29(8) 10_455 1_555 2_555
Ca1 Si1 Ca1 152.0(3) 10_554 1_555 10_455
Ca1 Si1 D 107.8(5) 10_554 1_555 10_555
Ca1 Si1 D 50.9(2) 10_554 1_555 10_554
Ca1 Si1 Si1 70.29(8) 10_554 1_555 2_554
Ca1 Si1 Si1 130.05(15) 10_554 1_555 2_555
Ca1 Si1 Ca1 94.73(7) 10_454 1_555 10_554
Ca1 Si1 Ca1 78.47(5) 10_454 1_555 10_455
Ca1 Si1 D 107.8(5) 10_454 1_555 10_555
Ca1 Si1 D 50.9(2) 10_454 1_555 10_554
Ca1 Si1 Si1 70.29(8) 10_454 1_555 2_554
Ca1 Si1 Si1 130.05(15) 10_454 1_555 2_555
Ca1 Si1 Ca1 152.0(3) 10_555 1_555 10_454
Ca1 Si1 Ca1 78.47(5) 10_555 1_555 10_554
Ca1 Si1 Ca1 94.73(7) 10_555 1_555 10_455
Ca1 Si1 D 50.9(2) 10_555 1_555 10_555
Ca1 Si1 D 107.8(5) 10_555 1_555 10_554
Ca1 Si1 Si1 130.05(15) 10_555 1_555 2_554
Ca1 Si1 Si1 70.29(8) 10_555 1_555 2_555
D Si1 Ca1 111.9(4) 1_455 1_555 10_555
D Si1 Ca1 45.3(3) 1_455 1_555 10_454
D Si1 Ca1 111.9(4) 1_455 1_555 10_554
D Si1 Ca1 45.3(3) 1_455 1_555 10_455
D Si1 D 62.73(14) 1_455 1_555 10_555
D Si1 D 62.73(14) 1_455 1_555 10_554
D Si1 Si1 115.5(3) 1_455 1_555 2_554
D Si1 Si1 115.5(3) 1_455 1_555 2_555
D Si1 D 94.1(11) 1_555 1_555 1_455
D Si1 Ca1 45.3(3) 1_555 1_555 10_555
D Si1 Ca1 111.9(4) 1_555 1_555 10_454
D Si1 Ca1 45.3(3) 1_555 1_555 10_554
D Si1 Ca1 111.9(4) 1_555 1_555 10_455
D Si1 D 62.73(14) 1_555 1_555 10_555
D Si1 D 62.73(14) 1_555 1_555 10_554
D Si1 Si1 115.5(3) 1_555 1_555 2_554
D Si1 Si1 115.5(3) 1_555 1_555 2_555
Ca1 Si1 D 47.0(6) 1_555 1_555 1_555
Ca1 Si1 D 47.0(6) 1_555 1_555 1_455
Ca1 Si1 Ca1 75.98(14) 1_555 1_555 10_555
Ca1 Si1 Ca1 75.98(14) 1_555 1_555 10_454
Ca1 Si1 Ca1 75.98(14) 1_555 1_555 10_554
Ca1 Si1 Ca1 75.98(14) 1_555 1_555 10_455
Ca1 Si1 D 47.7(7) 1_555 1_555 10_555
Ca1 Si1 D 47.7(7) 1_555 1_555 10_554
Ca1 Si1 Si1 129.2(2) 1_555 1_555 2_554
Ca1 Si1 Si1 129.2(2) 1_555 1_555 2_555
Ca1 D Ca1 110.0(16) 10_554 1_555 10_555
Ca1 D Ca1 103.7(2) 1_555 1_555 10_554
Ca1 D Ca1 103.7(2) 1_555 1_555 10_555
Ca1 D Ca1 131.4(18) 1_655 1_555 1_555
Ca1 D Ca1 103.7(2) 1_655 1_555 10_554
Ca1 D Ca1 103.7(2) 1_655 1_555 10_555
Si1 D Ca1 73.9(8) 10_554 1_555 1_655
Si1 D Ca1 73.9(8) 10_554 1_555 1_555
Si1 D Ca1 77.24(18) 10_554 1_555 10_554
Si1 D Ca1 172.7(15) 10_554 1_555 10_555
Si1 D Si1 95.5(14) 10_555 1_555 10_554
Si1 D Ca1 73.9(8) 10_555 1_555 1_655
Si1 D Ca1 73.9(8) 10_555 1_555 1_555
Si1 D Ca1 172.7(15) 10_555 1_555 10_554
Si1 D Ca1 77.24(18) 10_555 1_555 10_555
D D Si1 123.7(14) 10_654 1_555 10_555
D D Si1 66.2(8) 10_654 1_555 10_554
D D Ca1 50.2(5) 10_654 1_555 1_655
D D Ca1 137.1(9) 10_654 1_555 1_555
D D Ca1 53.5(7) 10_654 1_555 10_554
D D Ca1 117.8(16) 10_654 1_555 10_555
D D D 167(3) 10_555 1_555 10_654
D D Si1 66.2(8) 10_555 1_555 10_555
D D Si1 123.7(14) 10_555 1_555 10_554
D D Ca1 137.1(9) 10_555 1_555 1_655
D D Ca1 50.2(5) 10_555 1_555 1_555
D D Ca1 117.8(16) 10_555 1_555 10_554
D D Ca1 53.5(7) 10_555 1_555 10_555
D D D 97.8(5) 10_655 1_555 10_555
D D D 80.7(4) 10_655 1_555 10_654
D D Si1 66.2(8) 10_655 1_555 10_555
D D Si1 123.7(14) 10_655 1_555 10_554
D D Ca1 50.2(5) 10_655 1_555 1_655
D D Ca1 137.1(9) 10_655 1_555 1_555
D D Ca1 117.8(16) 10_655 1_555 10_554
D D Ca1 53.5(7) 10_655 1_555 10_555
D D D 167(3) 10_554 1_555 10_655
D D D 80.7(4) 10_554 1_555 10_555
D D D 97.8(5) 10_554 1_555 10_654
D D Si1 123.7(14) 10_554 1_555 10_555
D D Si1 66.2(8) 10_554 1_555 10_554
D D Ca1 137.1(9) 10_554 1_555 1_655
D D Ca1 50.2(5) 10_554 1_555 1_555
D D Ca1 53.5(7) 10_554 1_555 10_554
D D Ca1 117.8(16) 10_554 1_555 10_555
Si1 D D 118.3(17) 1_655 1_555 10_554
Si1 D D 51.1(9) 1_655 1_555 10_655
Si1 D D 118.3(17) 1_655 1_555 10_555
Si1 D D 51.1(9) 1_655 1_555 10_654
Si1 D Si1 117.27(14) 1_655 1_555 10_555
Si1 D Si1 117.27(14) 1_655 1_555 10_554
Si1 D Ca1 67.3(4) 1_655 1_555 1_655
Si1 D Ca1 161.4(14) 1_655 1_555 1_555
Si1 D Ca1 67.0(7) 1_655 1_555 10_554
Si1 D Ca1 67.0(7) 1_655 1_555 10_555
Si1 D Si1 94.1(11) 1_555 1_555 1_655
Si1 D D 51.1(9) 1_555 1_555 10_554
Si1 D D 118.3(17) 1_555 1_555 10_655
Si1 D D 51.1(9) 1_555 1_555 10_555
Si1 D D 118.3(17) 1_555 1_555 10_654
Si1 D Si1 117.27(14) 1_555 1_555 10_555
Si1 D Si1 117.27(14) 1_555 1_555 10_554
Si1 D Ca1 161.4(14) 1_555 1_555 1_655
Si1 D Ca1 67.3(4) 1_555 1_555 1_555
Si1 D Ca1 67.0(7) 1_555 1_555 10_554
Si1 D Ca1 67.0(7) 1_555 1_555 10_555
loop_
_geom_bond_atom_site_label_1
_geom_bond_atom_site_label_2
_geom_bond_distance
_geom_bond_site_symmetry_1
_geom_bond_site_symmetry_2
Ca1 D 2.38(2) 1_555 10_555
Ca1 D 2.38(2) 1_555 10_554
Ca1 D 2.491(16) 1_555 1_555
Ca1 D 2.491(16) 1_555 1_455
Ca1 Si1 3.0850(18) 1_555 10_455
Ca1 Si1 3.0850(18) 1_555 10_554
Ca1 Si1 3.0850(18) 1_555 10_454
Ca1 Si1 3.0850(18) 1_555 10_555
Ca1 Si1 3.139(8) 1_555 1_555
Si1 Si1 2.517(8) 1_555 2_555
Si1 Si1 2.517(8) 1_555 2_554
Si1 D 2.64(3) 1_555 10_554
Si1 D 2.64(3) 1_555 10_555
Si1 Ca1 3.0850(18) 1_555 10_455
Si1 Ca1 3.0850(18) 1_555 10_554
Si1 Ca1 3.0850(18) 1_555 10_454
Si1 Ca1 3.0850(18) 1_555 10_555
Si1 D 3.10(3) 1_555 1_455
Si1 D 3.10(3) 1_555 1_555
Si1 Ca1 3.139(8) 1_555 1_555
D Ca1 2.38(2) 1_555 10_555
D Ca1 2.38(2) 1_555 10_554
D Ca1 2.491(16) 1_555 1_555
D Ca1 2.491(16) 1_555 1_655
D Si1 2.64(3) 1_555 10_554
D Si1 2.64(3) 1_555 10_555
D D 3.012(12) 1_555 10_654
D D 3.012(12) 1_555 10_555
D D 3.012(12) 1_555 10_655
D D 3.012(12) 1_555 10_554
D Si1 3.10(3) 1_555 1_655
D Si1 3.10(3) 1_555 1_555
